Microstructure Evolution and Mechanical Properties .iv Microstructure Evolution and Mechanical...
Embed Size (px)
Transcript of Microstructure Evolution and Mechanical Properties .iv Microstructure Evolution and Mechanical...
THESIS FOR THE DEGREE OF DOCTOR OF PHILOSOPHY
Microstructure Evolution and Mechanical Properties
C E E N A J O S E P H
Department of Industrial and Materials Science CHALMERS UNIVERSITY OF TECHNOLOGY
Gteborg, Sweden, 2018
Microstructure Evolution and Mechanical Properties of Haynes 282 CEENA JOSEPH ISBN:978-91-7597-701-0 C e e n a J o s e p h , 2018 Doktorsavhandlingar vid Chalmers tekniska hgskola Ny serie nr 4382 ISSN 0346-718X
Department of Industrial and Materials Science Chalmers University of Technology SE-412 96 Gteborg Sweden Tel:+46 (0)31 772 1000 Printed by Chalmers Reproservice Gteborg, Sweden 2018
Adina & Alina
Microstructure Evolution and Mechanical Properties of Haynes 282
CEENA JOSEPH Department of Industrial and Materials Science
Chalmers University of Technology
Precipitation-hardened nickel-based superalloys find wide applications in aero engines and land-based gas turbines due to a combination of properties such as high temperature strength, resistance to oxidation and corrosion, fabricability, and creep strength. Structural engine components are traditionally cast to achieve higher degree of geometrical design freedom. However, the latest fabrication strategy to achieve low cost and light weight structural components is by joining materials based on temperature needs. The challenge in this strategy is to tailor the heat treatment to suit the multi-material structures and still be able to meet the desired property requirements. This requires a profound understanding of the process-structure-property relationships in these complex alloys. The newly introduced Ni-base superalloy Haynes 282 has been attracting interest due to its high-temperature properties and excellent weldability. These properties are achieved due to the precipitation of strengthening phase (, Ni3 (Al,Ti)) and grain boundary carbides (mainly M23C6 and M6C) during heat treatment.
As Haynes 282 has showed sensitivity to heat treatment temperatures within the typical tolerance limits around the conventional heat treatment, the main objective of this research was to understand the microstructural evolution and mechanical properties with changes in heat treatment conditions. The effect of heat treatment variations on microstructure and mechanical properties has been systematically studied. Its influence on microstructure and tensile properties between room temperature and 730 C are presented.
The results show that does not precipitate during rapid cooling but it precipitates as fine spherical particles during air cooling from the carbide stabilization temperature, and it changes to bimodal distribution with square and spherical morphology during slow cooling. During ageing, is seen to precipitate intergranularly, as well as along the grain boundaries. The solvus temperature for this phase was above 1010 C (higher than previously suggested), and depending on the combination of temperatures and times of the heat treatments, the morphology changes from spherical to bi-modal to cuboidal. The grain boundary carbide morphology depends strongly on heat treatment temperature and is seen to change from continuous film to brick wall structure and finally to discrete particles. These microstructural changes strongly affect both strength and ductility of the material.
Furthermore, Haynes 282 forgings show ductility variations in short transverse direction. The lower limit of ductility in this direction is close to the design tolerance and thus creates a need
to understand the underlying cause. In this part, the study is focused to understand ductility variation by microscopic investigations. Carbide segregation and banding is seen to influence the ductility when oriented perpendicular to the tensile axis. This influence is also qualitatively captured through micromechanical modelling.
Keywords: Haynes 282, gamma prime, carbides, isothermal transformation, anisotropy ductility, heat treatment, microstructure, solution treatment, carbide stabilization treatment
This licentiate thesis is based on the work performed at the Department of Industrial Materials Science (Previous Materials and Manufacturing Technology), Chalmers University of Technology during the period June 2012-Dec 2017. During this period the work was performed within the project funded by Swedish National Aeronautical Research Program (NFFP6) under the supervision of Professor Christer Persson and Docent Magnus Hrnqvist Colliander.
This thesis consists of an introductory part followed by the appended papers.
List of Appended papers
Paper I: Anisotropy of room temperature Ductility in Haynes 282 forgings
C. Joseph, M. Hrnqvist Colliander, C. Persson
Proceedings of the 8th International Symposium on Superalloy 718 and Derivatives, p. 601-609
Paper II: Influence of Carbide distribution on Ductility of Haynes 282 forgings
C. Joseph, M. Hrnqvist Colliander, R. Brommesson, C. Persson
13th International Symposium on Superalloys, SUPERALLOYS 2016, Seven Springs Mountain Resort Seven Springs, United States, 11 September 2016 through 15 September 2016, p. 523-529
Paper III: Influence of Heat treatments on the Microstructure and Tensile Properties of Haynes 282 sheet material
C. Joseph, C. Persson, M. Hrnqvist Colliander
Materials Science & Engineering A: Structural Materials: Properties, Microstructure and Processing. Vol. 679, p. 520-530
Paper IV: Gamma prime Precipitation in a Nickel base Superalloy during cooling
C. Joseph, M. Thuvander , J. Moverare , C. Persson and M. Hrnqvist Colliander
Submitted for journal publication
Paper V: Isothermal Phase Transformation in Nickel base Superalloy Haynes 282
C. Joseph, C. Persson and M. Hrnqvist Colliander
Submitted for journal publication
Paper VI: Microstructure and Mechanical Properties of Haynes 282 - Effect of variations in Solution Treatment
C. Joseph, S Sreekanth, B. Pettersson, C. Persson, M. Hrnqvist Colliander
Paper VII: Effect of Variations in Carbide Stabilization Treatment on Microstructure and Mechanical properties of Haynes 282
C. Joseph, M. Hrnqvist Colliander, B. Pettersson, C. Persson
Paper not appended to the thesis
Paper I: Dynamic strain aging in Haynes 282 superalloy
M. Hrnqvist Colliander, C. Joseph, C. Persson et al
Proceedings of the 2nd Euro Superalloys Conference. Vol. 14, p. Art. no. 16002-
Paper II: 3D grain structure modelling of intergranular fracture in forged Haynes 282
R. Brommesson, M. Ekh, C. Joseph
Engineering Fracture Mechanics. Vol. 154, p. 57-71
Contribution to the appended papers
My contribution to the appended papers is as follows
Paper I: The work was planned together with GKN aerospace. I did the microscopy work and wrote the paper in cooperation with the co-authors.
Paper II: The work was planned together with GKN aerospace. I did the microscopy work and the modelling part was done by Rebecka Brommesson. The paper was written by me with in cooperation with the co-authors.
Paper III: The work was planned by me in collaboration with my supervisors. The experimental work was performed by me. Mechanical testing was done by Prof. Christer Persson. The paper was written by me in cooperation with the co-authors.
Paper IV: The work was planned by me in collaboration with my supervisors. The preparation of the APT specimens was done by me with help from Dr.Mattias Thuvander. The APT experiments were performed by Dr. Mattias Thuvander. Modelling work was performed by J. Moverare and the paper was written by me in cooperation with the co-authors.
Paper V: The work was planned by me. The experimental work was performed by me. The paper was written by me in cooperation with the co-authors.
Paper VI: The work was planned by me. The microscopy work was performed by Suhas Sreekanth. Mechanical testing was done by Prof. Christer Persson. The paper was written by me in cooperation with the co-authors.
Paper VII: The work was planned and the experiments were performed by me. Mechanical testing was done by Prof. Christer Persson. The paper was written by me in cooperation with the co-authors.
List of Acronyms and Abbreviations
AC- Air cooled/ing
APT- Atom probe tomography
DSC-Differential scanning calorimetry
EBSD- Electron back scattered diffraction
EDS-Energy Dispersive x-ray spectroscopy
LSW-Lifschitz Slyozov Wagner
MA+A-Mill annealed +Aging
MA+LTA-Mill annealed + low temperature aging
PSD- Particle size distribution
SEM-Scanning electron Microscope
SHT- Standard Heat Treatment
ST+A- Solution treated + Aging
TTH- Time Temperature Hardness
TTT-Time Temperature Transformation
UTS-Ultimate tensile strength
Table of Contents
Chapter 1 .................................................................................................................................... 1